Molybdenum

42

niobium ← molybdenum → technetium


Cr
↑
Mo
↓
W




periodic table




General


Name, Symbol, Number

molybdenum, Mo, 42


Chemical series
transition metals


Group, Period, Block

6, 5, d


Appearance
gray metallic 



Atomic mass
95.94(2) g/mol


Electron configuration
[Kr] 4d5 5s1


Electrons per shell
2, 8, 18, 13, 1


Physical properties


Phase
solid


Density (near r.t.)
10.28 g/cm³


Liquid density at m.p.
9.33 g/cm³


Melting point
2896 K
(2623 °C, 4753 °F)


Boiling point
4912 K
(4639 °C, 8382 °F)


Heat of fusion
37.48 kJ/mol


Heat of vaporization
617 kJ/mol


Heat capacity
(25 °C) 24.06 J/(mol·K)




Vapor pressure


P/Pa
1
10
100
1 k
10 k
100 k


at T/K
2742
2994
3312
3707
4212
4879



Atomic properties


Crystal structure
cubic body centered


Oxidation states
2, 3, 4, 5, 6
(strongly acidic oxide)


Electronegativity
2.16 (Pauling scale)


Ionization energies
(more)

1st: 684.3 kJ/mol


2nd: 1560 kJ/mol


3rd: 2618 kJ/mol


Atomic radius
145 pm


Atomic radius (calc.)
190 pm


Covalent radius
145 pm


Miscellaneous


Magnetic ordering
no data


Electrical resistivity
(20 °C) 53.4 nΩ·m


Thermal conductivity
(300 K) 138 W/(m·K)


Thermal expansion
(25 °C) 4.8 µm/(m·K)


Speed of sound (thin rod)
(r.t.) 5400 m/s


Speed of sound (thin rod)
(r.t.) 329 m/s


Shear modulus
20 GPa


Bulk modulus
230 GPa


Poisson ratio
0.31


Mohs hardness
5.5


Vickers hardness
1530 MPa


Brinell hardness
1500 MPa


CAS registry number
7439-98-7


Notable isotopes




Main article: Isotopes of Molybdenum


iso

NA

half-life

DM

DE (MeV)

DP


92Mo

14.84%

Mo is stable with 50 neutrons


93Mo

syn

4×103 y

ε

-

93Nb


94Mo

9.25%

Mo is stable with 52 neutrons


95Mo

15.92%

Mo is stable with 53 neutrons


96Mo

16.68%

Mo is stable with 54 neutrons


97Mo

9.55%

Mo is stable with 55 neutrons


98Mo

24.13%

Mo is stable with 56 neutrons


99Mo

syn

65.94 h

β-

0.436, 1.214

99Tc


γ

0.74, 0.36,
0.14

-


100Mo

9.63%

7.8×1018 y

β-β-

?

100Ru


Molybdenum (chemical symbol Mo, atomic number 42) is a silvery white, soft metal. It has one of the highest melting points of all pure elements. It is used mainly in alloys, especially to make high-strength and high-temperature steels. It is also a catalyst in the petroleum industry. Molybdenum disulfide is a good lubricant, and molybdenum pigments are used in paints, inks, plastics, and rubber compounds. Molybdenum in trace amounts has been found to have a role in the biology of all classes of organisms. If ingested in excess, however, molybdenum dust and its water-soluble compounds can be toxic.

Contents

1 Occurrence
2 History
3 Notable characteristics

3.1 Isotopes


4 Compounds
5 Applications
6 Biological role
7 Precautions
8 Notes
9 See also
10 References
11 External links
12 Credits



Occurrence
The element molybdenum (from the Greek molybdos, meaning "lead-like") is not found free in nature. The main commercial source of molybdenum is the mineral molybdenite (MoS2), but it is also found in minerals such as wulfenite (PbMoO4) and powellite (CaMoO4).
Molybdenum is obtained by mining molybdenite directly and is also recovered as a byproduct of copper mining. Molybdenum is present in ores from 0.01 percent to about 0.5 percent. About half of the world's molybdenum is mined in the United States.
The Russian Luna 24 mission discovered a single grain (1 × 0.6 micrometer) of pure molybdenum in a pyroxene fragment taken from Mare Crisium on the Moon.

History
Until the late eighteenth century, the compounds of molybdenum were confused with those of other elements, such as carbon or lead. In 1778, Carl Wilhelm Scheele was able to determine that molybdenum was separate from graphite and lead, and he isolated the oxide of the metal from molybdenite. In 1782, Hjelm isolated an impure extract of the metal by reducing the oxide with carbon. Molybdenum was little used and remained in the laboratory until the late nineteenth century. Subsequently, a French company (Schneider and Co.) tried molybdenum as an alloying agent in steel armor plating and noted its usefulness as a hardener of steel. Molybdenum use soared during World War I, when the increased demand for tungsten made that element scarce and high-strength steels were at a premium.

Notable characteristics
Molybdenum is a transition metal that lies in period five of the periodic table, between niobium and technetium. In addition, it is located in group six (former group 6B), between chromium and tungsten.
Pure molybdenum has a melting point of 2623°C, which is among the highest melting points of all elements. The pure metal has a tendency to flake apart during machining, but it is useful as an additive that hardens steel.

Isotopes
Molybdenum has six stable isotopes and many radioisotopes, most of which have very short half-lives. Mo-99 is used to create Tc-99 for the nuclear isotope industry.

Compounds
Ammonium tetrathiomolybdate ((NH4)2MoS4): This bright red ammonium salt is an important reagent in the chemistry of molybdenum and has been used as a building block in bioinorganic chemistry. The thiometallate anion (MoS4-2) has the distinctive property of undergoing oxidation at the sulfur centers, concomitant with reduction of the metal from Mo(VI) to Mo(IV).
Molybdic acid: It refers to hydrated forms of molybdenum trioxide. The simplest form is the monohydrate, H2MoO4, but the dihydrate is also found. The salts of molybdic acid are called molybdates. As molybdenum can have various oxidation states, it can form a wide variety of salts.
Sodium molybdate (Na2MoO4): It is often found as the dihydrate (Na2MoO4 . 2H2O) and is useful as a source of molybdenum. It is also used in biochemistry and medicinal chemistry to track various colorless organic chemicals that, in the presence of the salt, can be stained blue. The blue color, also called molybdenum blue, is a complex of molybdates (Mo(VI), Mo(V)).
Molybdenum disulfide or molybdenum sulfide or molybdenum(IV) sulfide (MoS2): This black, crystalline sulfide occurs as the mineral molybdenite. Its structure, appearance, and feel are similar to graphite. It consists of a sandwich of layers of molybdenum atoms between layers of sulfur atoms. The weak interactions between the sheets gives MoS2 a lubricating effect. Finely powdered MoS2 is a common dry lubricant. It is also often mixed into various oils and greases, which allows the lubricated parts to keep running for a while beyond the almost complete loss of oil. It is used in aircraft engines, constant-velocity joints and universal joints in automobiles, and as a lubricating additive to special plastics, notably nylon and teflon. Synthetic MoS2 is a catalyst for desulfurization in petroleum refineries.[1]
Applications
Over two-thirds of all molybdenum is used in alloys, especially to make high-strength and high-temperature steels. Such alloys are used for oil pipelines, aircraft and missile parts, and filaments. Special alloys (such as the Hastelloys) are notably heat-resistant and corrosion-resistant.
Molybdenum also finds use as a catalyst in the petroleum industry, especially in catalysts for removing organic sulfurs from petroleum products.
It is used to form the anode in some X-ray tubes, particularly in mammography applications.
It is found in some electronics applications as the conductive metal layers in thin-film transistors (TFTs).
Molybdenum disulfide is a good lubricant, especially at high temperatures.
The isotope Mo-99 is used in the nuclear isotope industry.
Molybdenum pigments, ranging in color from red-yellow to a bright red-orange, are used in paints, inks, plastics, and rubber compounds.
Biological role
Molybdenum has been found to have a role in the biology of all classes of organisms. It is found in two groups of enzymes—the nitrogenases and the molybdopterins.
The nitrogenases are found in bacteria (that may dwell in plants) and are involved in the pathways of nitrogen fixation. The molybdenum atom is present in a cluster that includes iron and sulfur atoms. The name molybdopterin is misleading, as this group of enzymes includes tungsten-containing enzymes, and the word "molybdopterin" does not actually refer to the metal atom. This group may also be referred to as "mononuclear molybdenum enzymes," as the metal atom is not present in a cluster. These enzymes are involved in various processes that are part of the global sulfur, nitrogen, and carbon cycles.
There is a requirement for trace amounts of molybdenum in plants, and soils can be barren on account of molybdenum deficiencies. Plants and animals generally have molybdenum present in amounts of a few parts per million. In animals, molybdenum is a cofactor of the enzyme xanthine oxidase, which is involved in certain metabolic pathways (purine degradation and formation of uric acid). In some animals, adding a small amount of dietary molybdenum enhances growth.

Precautions
Molybdenum dusts and some molybdenum compounds, such as molybdenum trioxide and water-soluble molybdates, may have slight toxicities if inhaled or ingested orally. Laboratory tests suggest, however, that molybdenum is of relatively low toxicity, compared to many heavy metals. Acute toxicity in humans is unlikely, because the dose required would be exceptionally high. There is the potential for molybdenum exposure in mining and refining operations, as well as the chemical industry, but to date, no instance of harm from this exposure has been reported. Also, water-insoluble molybdenum compounds, such as the lubricant molybdenum disulfide, are considered nontoxic.
In ruminants, molybdenum toxicity occurs if the animals are allowed to graze on soil that is rich in molybdenum but deficient in copper. The molybdenum causes excretion of copper reserves from the animal, leading to copper deficiency. In young calves, the molybdenum toxicity is manifested as "teart" or shooting diarrhea, where the dung is watery, full of air bubbles and with a fetid odor. In pigs and sheep, molybdenum toxicity combined with copper deficiency can lead to a condition called sway back or paralysis of hind quarters. In black-coated animals, the toxicity of this metal is characterized by depigmentation of the skin surrounding the eyes, often referred to as "spectacled eyes."
Regulations by the U.S. Occupational Safety and Health Administration (OSHA) specify maximum molybdenum exposure in an eight-hour day (40-hour week) to be 15 milligrams (mg) per cubic meter. The National Institute for Occupational Safety and Health (NIOSH) recommends exposure limit of 5,000 mg per cubic meter.

Notes

↑  Hydrodesulfurization 


See also
Chemical element
Metal
Periodic table
Transition metal
ReferencesISBN links support NWE through referral fees
Chang, Raymond. Chemistry (ninth ed.) New York: McGraw-Hill Science/Engineering/Math, 2006. ISBN 0073221031
Cotton, F. Albert, and Geoffrey Wilkinson. Advanced Inorganic Chemistry (4th ed.), New York: Wiley, 1980. ISBN 0-471-02775-8
Greenwood, N.N.; and A. Earnshaw. Chemistry of the Elements (2nd Edition). Oxford, U.K.; Burlington, Massachusetts: Butterworth-Heinemann, Elsevier Science, 1998. ISBN 0750633654. Online version available at Knovel. Retrieved August 24, 2007.
Molybdenum Los Alamos National Laboratory. Retrieved August 24, 2007.
Topsøe, H., B. S. Clausen, and F. E. Massoth. Hydrotreating Catalysis, Science and Technology. Berlin: Springer-Verlag, 1996.
External links
All links retrieved November 9, 2022.

WebElements.com – Molybdenum.

Credits
New World Encyclopedia writers and editors rewrote and completed the Wikipedia article
in accordance with New World Encyclopedia standards. This article abides by terms of the Creative Commons CC-by-sa 3.0 License (CC-by-sa), which may be used and disseminated with proper attribution. Credit is due under the terms of this license that can reference both the New World Encyclopedia contributors and the selfless volunteer contributors of the Wikimedia Foundation. To cite this article click here for a list of acceptable citing formats.The history of earlier contributions by wikipedians is accessible to researchers here:

Molybdenum  history
Ammonium_tetrathiomolybdate  history
Molybdic_acid  history
Sodium_molybdate  history
Molybdenum_disulfide  history
The history of this article since it was imported to New World Encyclopedia:

History of "Molybdenum"
Note: Some restrictions may apply to use of individual images which are separately licensed.